text: The reduced vacancy concentration in nanocrystals can negatively affect the motion of dislocations, since dislocation climb requires vacancy migration. In addition, there exists a very high internal pressure due to the surface stress present in small nanoparticles with high radii of curvature. This causes a lattice strain that is inversely proportional to the size of the particle, also well known to impede dislocation motion, in the same way as it does in the work hardening of materials. For example, gold nanoparticles are significantly harder than the bulk material. Furthermore, the high surface-to-volume ratio in nanoparticles makes dislocations more likely to interact with the particle surface. In particular, this affects the nature of the dislocation source and allows the dislocations to escape the particle before they can multiply, reducing the dislocation density and thus the extent of plastic deformation.
  There are unique challenges associated with the measurement of mechanical properties on the nanoscale, as conventional means such as the universal testing machine cannot be employed. As a result, new techniques such as nanoindentation have been developed that complement existing electron microscope and scanning probe methods. Atomic force microscopy (AFM) can be used to perform nanoindentation to measure hardness, elastic modulus, and adhesion between nanoparticle and substrate. The particle deformation can be measured by the deflection of the cantilever tip over the sample. The resulting force-displacement curves can be used to calculate elastic modulus. However, it is unclear whether particle size and indentation depth affect the measured elastic modulus of nanoparticles by AFM.
  Adhesion and friction forces are important considerations in nanofabrication, lubrication, device design, colloidal stabilization, and drug delivery. The capillary force is the main contributor to the adhesive force under ambient conditions. The adhesion and friction force can be obtained from the cantilever deflection if the AFM tip is regarded as a nanoparticle. However, this method is limited by tip material and geometric shape. The colloidal probe technique overcomes these issues by attaching a nanoparticle to the AFM tip, allowing control oversize, shape, and material. While the colloidal probe technique is an effective method for measuring adhesion force, it remains difficult to attach a single nanoparticle smaller than 1 micron onto the AFM force sensor.
  Another technique is in situ TEM, which provides real-time, high resolution imaging of nanostructure response to a stimulus. For example, an in situ force probe holder in TEM was used to compress twinned nanoparticles and characterize yield strength. In general, the measurement of the mechanical properties of nanoparticles is influenced by many factors including uniform dispersion of nanoparticles, precise application of load, minimum particle deformation, calibration, and calculation model.
  Like bulk materials, the properties of nanoparticles are materials dependent. For spherical polymer nanoparticles, glass transition temperature and crystallinity may affect deformation and change the elastic modulus when compared to the bulk material. However, size-dependent behavior of elastic moduli could not be generalized across polymers. As for crystalline metal nanoparticles, dislocations were found to influence the mechanical properties of nanoparticles, contradicting the conventional view that dislocations are absent in crystalline nanoparticles.